Flexure test methods
The three fundamental mechanical property characterization tests of materials are tension, compression and shear. Note that flexure is not included. This article addresses some of the reasons why. When a beam resting on supports near its ends is loaded, the supported side is in tension and the opposite side is in
The three fundamental mechanical property characterization tests of materials are tension, compression and shear. Note that flexure is not included. This article addresses some of the reasons why.
When a beam resting on supports near its ends is loaded, the supported side is in tension and the opposite side is in compression. These induced bending stresses vary through the thickness of the beam. In addition, a shear stress is induced, which also varies through the thickness. All of these stresses also can vary along the length of the beam, with stress concentrations being introduced at the load and support points. As a further complication, the ratio of the magnitude of the normal (tensile and compressive) stresses to the shear stresses varies with the support span lengthtospecimen thickness ratio of the particular beam geometry being tested. Definitely, the stress state in a beam is far from the uniform state desired for material characterization.
Featured Content
The question thus arises, "Why are flexure tests conducted?" One reason is that, if the flexural loading adequately simulates the actual loading conditions the material will be subjected to in service, such a test can be very meaningful. Too often, unfortunately, the reason the test is conducted is that it is simple to perform, and little consideration is given to whether or not it is meaningful.
There are currently two ASTM standards governing flexural testing, ASTM D 790^{1} and ASTM D 6272^{2}. A third is currently being drafted^{3}. The first two are under the jurisdiction of ASTM Committee D20Plastics, while the draft standard is being prepared by ASTM Committee D30Composites. This leads to the next question, Why are three ASTM standards necessary?
ASTM D 790 has been in existence since 1970 and is well known. Until the late 1990s, this standard included both three and fourpoint loading. But then Committee D20 eliminated fourpoint loading from ASTM D 790, creating much concern among Committee D30 members and the associated composite materials community, who routinely used this standard for both threepoint and fourpoint loading. As a compromise, Committee D20 then issued a new standard, ASTM D 6272, which included only fourpoint loading.
Committee D30, to protect its future interests, decided to write its own standard, to include both three and fourpoint loading. This effort was initiated approximately five years ago, and while the draft standard is still being revised and balloted, it appears, finally, to be nearing completion.
As noted above, both three and fourpoint loadings are commonly used. This terminology, while universally used, can be a bit confusing. In both cases, the beam to be tested is simply supported near each end, the distance between these supports being termed the support span. The beam is then either loaded at midspan (threepoint loading) or at two positions equidistant from the two supports (fourpoint loading). While the distance of these two loading positions from the supports could be arbitrarily selected, as will be discussed, the corresponding ASTM documents specify the distance to be either onefourth or onethird of the support span, referred to, respectively as quarterpoint or thirdpoint loading.
Fig. 1 indicates the three standard beam configurations. The loading magnitudes shown are those required to induce the same maximum bending moment in each beam.
When these configurations are compared, the significant parameters are the total loading applied to each configuration to achieve the same maximum bending moment in the beam, and the corresponding maximum local forces and maximum induced shear forces. These comparisons are shown in Table 1.
Note that to achieve an equal bending moment, twice as much total force must be applied to the quarterpoint loaded beam, and 1.5 times as much to the thirdpoint loaded beam. However, this is usually of little consequence in terms of testing machine capacity, since the required loadings are typically relatively low for flexural testing.
Of greater interest is the magnitude of the maximum local force, since this induces local stress concentrations in the beam and, possibly, degraded flexural strength. Thirdpoint loading is the most favorable. Likewise, it is desirable to minimize the maximum shear force, to reduce the possibility of inducing unwanted shear failures in the beam, which would invalidate the flexure test results. Threepoint loading is superior in this case.
One interesting extrapolation is that if the loading points are progressively moved even closer to the center of the beam, as they approach the limit (of becoming a single central force) the maximum local force and the maximum shear force both approach 1/2 P ("P" represents the applied load). That is, if the beam were loaded by two discrete forces near the center of the beam, the maximum local force would approach onehalf that in the threepoint loaded beam and the maximum shear force would be no higher than for threepoint loading. This also suggests that threepoint loading is also a favorable configuration, but that the central loading should be spread out to avoid high local stress concentrations.
One additional consideration should be noted. For threepoint loading, the maximum bending moment occurs only at the center of the beam. For fourpoint loading, the bending moment is uniformly maximum between the loading points. That is, a greater volume of the beam is subjected to the maximum bending moment. But even this factor is tempered somewhat by the fact that the local stress concentrations can still make the loading point locations the critical sections.
Finally, the length of the beam must be selected. This is typically specified as the ratio of the support span length (s) to the beam thickness (t). The two existing ASTM standards recommend a ratio of 16:1 while the draft document specifies 32:1. However, since the induced shear stresses decrease relative to the bending moment as s/t increases, all three documents permit increasing this ratio if necessary to reduce shear effects, and all cite ratios of 16:1, 32:1, 40:1 and 60:1. Incidentally, the use of these specific ratios has no special significance, their selection being driven more by historical than technical considerations. Some guidelines for selecting an appropriate ratio are presented in the ASTM documents.
What then can be concluded from this discussion? Of the three standard loading configurations, threepoint loading has definite advantages, particularly if the concentrated loading can be spread out a bit. One way to spread the loading is to use a larger loading radius. Currently both existing ASTM standards specify 5 mm (0.197 inch) radii, while the ASTM draft document specifies 3.2 mm (0.125 inch). The present discussion suggests that even larger radii would be beneficial in all cases.
References
^{1}ASTM Standard D 79003, "Test Methods for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials," ASTM International, W. Conshohocken, Pa. (first issued in 1970).
^{2}ASTM Standard D 627202, "Test Method for Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials by FourPoint Bending," ASTM International, W. Conshohocken, Pa. (first issued in 1998).
^{3}ASTM Draft Standard, "Standard Test Methods for Flexural Properties of FiberReinforced Polymer Matrix Composites," ASTM International, W. Conshohocken, Pa. (in preparation).
Related Topics
RELATED CONTENT

Outofautoclave processing: <1% void content?
Research sheds light on air and airbubble behavior in OOA aerospace prepregs.

Shear test methods: Iosipescu vs. VNotched Rail
Dr. Don Adams asks and suggests a likely answer to the question Which shear test method is best?

Impact testing of composite materials
Dr. Donald F. Adams (Wyoming Test Fixtures (Salt Lake City, Utah) discusses the methods for impact testing of composites.